# Ti3O5/SiO2 다층박막를 이용한 협대역 칼라투과필터 제작 및 특성연구

• Accepted : 2011.12.17
• Published : 2011.12.31

#### Abstract

Purpose: The narrow-band pass color-filters with a 500 nm central wavelength and 12 nm FWHM using $Ti_3O_5/SiO_2$ mutilayer were fabricated, and their characteristics and structures were studied. Methods: the optical constants, n and k, of the $Ti_3O_5$ and $SiO_2$ thin films were obtained from the transmittances of their thin film. The narrow-band pass color-filters were designed with these optical constants and the AR coating of the filter was also designed. $Ti_3O_5/SiO_2$ multilayer filters were made by electron beam evaporation apparatus and the transmittaces of the filters were measured by spectrophotometer. the number of layers and the thicknesses of filters were calculated from the cross section of filters by SEM image and the composition of filters was analysed by XPS analysis. Results: The optimization of AR coating for the narrow-band pass color-filter was [air$|SiO_2(90)|Ti_3O_5(36)|SiO_2(5)|Ti_3O_5(73)|SiO_2(30)|Ti_3O_5(15)|$ glass], and the optimization of filter layer for the color filter was [air$|SiO_2(192)|Ti_3O_5(64)|SiO_2(102)|Ti_3O_5(66)|SiO_2(112)|Ti_3O_5(74)|SiO_2(120)|Ti_3O_5(68)|SiO_2(123)|Ti_3O_5(80)|SiO_2(109)|Ti_3O_5(70)|SiO_2(105)|Ti_3O_5(62)|SiO_2(99)|Ti_3O_5(63)|SiO_2(98)|Ti_3O_5(51)|SiO_2(60)|Ti_3O_5(42)|SiO_2(113)|Ti_3O_5(88)|SiO_2(116)|Ti_3O_5(68)|SiO_2(89)|Ti_3O_5(49)|SiO_2(77)|Ti_3O_5(48)|SiO_2(84)|Ti_3O_5(51)|SiO_2(85)|Ti_3O_5(48)|SiO_2(59)|Ti_3O_5(34)|SiO_2(71)|Ti_3O_5(44)|SiO_2(65)|Ti_3O_5(45)|SiO_2(81)|Ti_3O_5(52)|SiO_2(88)|$ glass]. It was known that the color-filters fabricated by the simulation data were composed of 41 layers by SEM image and the top layer of filters was $SiO_2$ layer and the filters were composed of $SiO_2$/$Ti_3O_5$ multilayer by XPS analysis. It was also known that the mixed thin film of TiO2 and $Ti_3O_5$ was made during the deposition of the $Ti_3O_5$ material. Conclusions: The narrow-band pass color-filters with a 500 nm central wavelength and 12 nm FWHM using $Ti_3O_5/SiO_2$ mutilayer of 41 layer were fabricated, and it was known that the mixed form of TiO2 and $Ti_3O_5$ thin film was made during the deposition of the $Ti_3O_5$ material.

#### References

1. (주)한국산업정보센터, "다층코팅박막기술: 레이저 기술 자료"(2005), http://www.dienmold.com/tooling/view.asp?idx=36&table=laser_9(2005.07.07.).
2. Alfred Thelen, "Design of Optical Interference Coatings", 1st ed., McGraw-Hill, New York, U.S.A., pp.157-176 (1988).
3. 황보창권, "박막광학", 초판, 다성출판사, 서울, pp.301-328(2000).
4. H. A. Macleod, "Thin-film optical filters", 2nd ed., Macmillan, New York, U.S.A., pp.234-311(1986).
5. 하늘기획, "행성관측용필터", 제품상세정보(2011), http://www.sky39.com/product.htm?mode=product_view&goods_code=3098&site=default(2011.10.31.)
6. 황보창권, 진권휘, 박대윤, 이민희, "포락선 방법을 이용한 흡수가 작은 박막의 광학 상수 및 두께 결정", The Journal of Optical Society of Korea, 3(1):1-10(1992).
7. 박문찬, 김동진, "$Ti_3O_5/SiO_2$ 다층박막를 이용한 협대역 칼라투과필터 설계", 신흥대학 부설 보건과학연구소논문집, 15:55-66(2011).